# 1 Introduction to Crystalline Anisotropy and the Crystal ... . Crystal Plasticity Finite Element...

date post

14-May-2018Category

## Documents

view

213download

0

Embed Size (px)

### Transcript of 1 Introduction to Crystalline Anisotropy and the Crystal ... . Crystal Plasticity Finite Element...

Franz~Roters, Philip~Eisenlohr, Thomas~R.~Bieler, and~Dierk~Raabe: Crystal Plasticity Finite Element Methods Chap. roters9419c01 2010/7/28 page 1 le-tex

1

1Introduction to Crystalline Anisotropyand the Crystal Plasticity Finite Element Method

Crystalline matter is mechanically anisotropic. This means that the instantaneousand time-dependent deformation of crystalline aggregates depends on the directionof the mechanical loads and geometrical constraints imposed. This phenomenonis due to the anisotropy of the elastic tensor, Figure 1.1, and to the orientationdependence of the activation of the crystallographic deformation mechanisms (dis-locations, twins, martensitic transformations), Figure 1.2.

An essential consequence of this crystalline anisotropy is that the associated me-chanical phenomena such as material strength, shape change, ductility, strain hard-ening, deformation-induced surface roughening, damage, wear, and abrasion arealso orientation-dependent. This is not a trivial statement as it implies that me-chanical parameters of crystalline matter are generally tensor-valued quantities.Another major consequence of the single-crystal elastic-plastic anisotropy is that itadds up to produce also macroscopically directional properties when the orienta-tion distribution (crystallographic texture) of the grains in a polycrystal is not ran-dom. Figure 1.3a,b shows such an example of a plain carbon steel sheet with a pre-ferred crystal orientation (here high probability for a crystallographic f111g planebeing parallel to the sheet surface) after cup drawing. Plastic anisotropy leads tothe formation of an uneven rim (referred to as ears or earing) and a heterogeneous

Figure 1.1 Elastic anisotropy in a polycrystal resulting from superposition of single-crystalanisotropy.

Crystal Plasticity Finite Element Methods.Franz Roters, Philip Eisenlohr, Thomas R. Bieler, and Dierk RaabeCopyright 2010 WILEY-VCH Verlag GmbH & Co. KGaA, WeinheimISBN: 978-3-527-32447-7

Franz~Roters, Philip~Eisenlohr, Thomas~R.~Bieler, and~Dierk~Raabe: Crystal Plasticity Finite Element Methods Chap. roters9419c01 2010/7/28 page 2 le-tex

2 1 Introduction to Crystalline Anisotropy and the Crystal Plasticity Finite Element Method

Figure 1.2 Plastic anisotropy in a single crystal due to distinct crystallography.

Figure 1.3 Consequence of plastic anisotropywhen drawing a textured sheet into a cup. Theorientation distribution before deformation ex-hibits a high volume fraction of grains with a

crystallographic [111] axis parallel to the sheetnormal. The arrows in (a) mark six ears result-ing from preferential material flow. (b) Thecorresponding crystal plasticity finite elementsimulation.

distribution of material thinning during forming. It must be emphasized in thatcontext that a random texture is not the rule but a rare exception in real materials.In other words, practically all crystalline materials reveal macroscopic anisotropy.

Franz~Roters, Philip~Eisenlohr, Thomas~R.~Bieler, and~Dierk~Raabe: Crystal Plasticity Finite Element Methods Chap. roters9419c01 2010/7/28 page 3 le-tex

1 Introduction to Crystalline Anisotropy and the Crystal Plasticity Finite Element Method 3

A typical example of such macroscopic anisotropy is the uniaxial stressstraincurve, which is the most important mechanical measure in the design of structuralmaterials. The introductory statement made above implies that uniaxial stressstrain curves represent an incomplete description of plastic deformation as theyreduce a six-dimensional yield surface and its change upon loading to a one-dimen-sional (scalar) yield curve, see Figure 1.4. Another consequence of this statement isthat the crystallographic texture (orientation distribution) and its evolution duringforming processes is a quantity that is inherently connected with plasticity theo-ry, more precisely, with the anisotropy of the underlying plasticity mechanisms.Texture can, hence, be used to describe the integral anisotropy of polycrystals interms of the individual tensorial behavior of each grain and the orientation-depen-dent boundary conditions among the crystals. Formally, the connection betweenshear and texture evolution becomes clear from the fact that any deformation gra-dient can be expressed as the combination of its skew-symmetric portion, whichrepresents a pure rotation leading to texture changes if not matched by the rota-tion implied by plastic shear, and a symmetric tensor that is a measure of purestretching. Plastic shear, hence, creates both shape and orientation changes, exceptfor certain highly symmetric shears. Therefore, a theory of the mechanical prop-erties of crystals must include, first, the crystallographic and anisotropic natureof those mechanisms that create shear and, second, the orientation(s) of the crys-

Figure 1.4 Flow stress and strain hardening of anisotropic materials are tensor quantities.

Franz~Roters, Philip~Eisenlohr, Thomas~R.~Bieler, and~Dierk~Raabe: Crystal Plasticity Finite Element Methods Chap. roters9419c01 2010/7/28 page 4 le-tex

4 1 Introduction to Crystalline Anisotropy and the Crystal Plasticity Finite Element Method

tal(s) studied relative to the boundary conditions applied (e.g., loading axis, rollingplane).

Early approaches to describe anisotropic plasticity under simple boundary con-ditions considered these aspects, such as the Sachs (1928), Taylor (1938), BishopHill, and Krner (1961) formulations. However, these approaches were neither de-signed for considering explicitly the mechanical interactions among the crystals ina polycrystal nor for responding to complex internal or external boundary condi-tions, see Figure 1.5ad. Instead, they are built on certain simplifying assumptionsof strain or stress homogeneity to cope with the intricate interactions within a poly-crystal.

For that reason variational methods in the form of finite element approximationshave gained enormous momentum in the field of crystal mechanical modeling.These methods, which are referred to as crystal plasticity finite element (CPFE)models, are based on the variational solution of the equilibrium of the forces andthe compatibility of the displacements using a weak form of the principle of virtualwork in a given finite-volume element. The entire sample volume under consider-ation is discretized into such elements. The essential step which renders the defor-mation kinematics of this approach a crystal plasticity formulation is the fact thatthe velocity gradient is written in dyadic form. This reflects the tensorial crystal-lographic nature of the underlying defects that lead to shear and, consequently, toboth shape changes (symmetric part) and lattice rotations (skew-symmetric part),see Chapter 3. This means that the CPFE method has evolved as an attempt toemploy some of the extensive knowledge gained from experimental and theoret-ical studies of single-crystal deformation and dislocations to inform the furtherdevelopment of continuum field theories of deformation. The general frameworksupplied by variational crystal plasticity formulations provides an attractive vehi-cle for developing a comprehensive theory of plasticity that incorporates existingknowledge of the physics of deformation processes (Arsenlis et al., 2004; Curtinand Miller, 2003; Vitek, Mrovec, and Bassani, 2004a) into the computational toolsof continuum mechanics (Zienkiewicz, 1967; Zienkiewicz and Taylor, 2005) withthe aim to develop advanced and physically based design methods for engineeringapplications (Zhao et al., 2004a).

One main advantage of CPFE models lies in their capability to solve crystalmechanical problems under complicated internal and/or external boundary con-ditions. This aspect is not a mere computational advantage, but it is an inher-ent part of the physics of crystal mechanics since it enables one to tackle thoseboundary conditions that are imposed by inter- and intragrain micro-mechanicalinteractions, Figure 1.6 (Sachtleber, Zhao, and Raabe, 2002). This is not only es-sential to study in-grain or grain cluster mechanical problems but also to betterunderstand the often quite abrupt mechanical transitions at interfaces (Raabe etal., 2003).

However, the success of CPFE methods is not only built on their efficiency indealing with complicated boundary conditions. They also offer high flexibility withrespect to including various constitutive formulations for plastic flow and hard-ening at the elementary shear system level. The constitutive flow laws that were

Franz~Roters, Philip~Eisenlohr, Thomas~R.~Bieler, and~Dierk~Raabe: Crystal Plasticity Finite Element Methods Chap. roters9419c01 2010/7/28 page 5 le-tex

1 Introduction to Crystalline Anisotropy and the Crystal Plasticity Finite Element Method 5

Figure 1.5 The increasing complexity of crys-tal-scale micromechanics with respect to theequilibrium of the forces and the compatibilityof the displacements for different situations:(a, b) Single-slip situation in a single crystalpresented in stress space. (c) Portion of asingle-crystal yield surface with three slip sys-tems. (d) Multislip situation in a polycrystal

where all different crystals have to satisfy anassumed imposed strain in their respectiveyield corners. If the strain is homogeneous,this situation leads to different stresses ineach crystal (Raabe et al., 2002a, 2004a). crit :critical shear stress; TBH: TaylorBishopHillstress state (stress required to reach a yieldcorner).

suggested during the last few decades have gradually developed from empiricalviscoplastic formulations (Asaro and Rice, 1977; Rice, 1971) into microstructure-based multiscale models of plasticity including a variety of size-dependent effectsand interface mechanisms (Arsenlis and Parks, 1999, 2002; Arsenlis et

*View more*